Deformations of the α-Fe~2~O~3~ rhombohedral lattice across the Néel temperature
Fabrykiewicz, P.; Stekiel, M.; Sosnowska, I.; Przeniosło, R.; Acta Crystallographica Section B 73 (2017) 27–32; doi:10.1107/S2052520616017935

data_2108028
_publ_section_title
;
 Deformations of the \a-Fe~2~O~3~ rhombohedral lattice across the N\'eel
 temperature
;
_journal_coeditor_code           DQ5016
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              27
_journal_page_last               32
_journal_paper_doi               10.1107/S2052520616017935
_journal_volume                  73
_journal_year                    2017
_chemical_formula_sum            'Fe2 O3'
_chemical_formula_weight         159.7
_chemical_name_common            hematite
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 162.3508(2)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.68920(8)
_cell_length_b                   5.08737(2)
_cell_length_c                   13.84868(11)
_cell_measurement_reflns_used    935
_cell_measurement_temperature    1053
_cell_measurement_theta_max      30.0
_cell_measurement_theta_min      5.0
_cell_volume                     206.967(3)
_diffrn_ambient_temperature      1053
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     0.40086
_exptl_crystal_density_diffrn    5.1249
_exptl_crystal_F_000             304
_pd_meas_2theta_range_inc        0.001
_pd_meas_2theta_range_max        48.002
_pd_meas_2theta_range_min        5.000
_pd_meas_number_of_points        43003
_pd_proc_2theta_range_inc        0.001
_pd_proc_2theta_range_max        29.999
_pd_proc_2theta_range_min        5
_pd_proc_ls_background_function  '5 Legendre polynoms'
_pd_proc_ls_pref_orient_corr     none
_pd_proc_ls_profile_function     Pseudo-Voigt
_pd_proc_ls_prof_R_factor        0.0988
_pd_proc_ls_prof_wR_expected     0.0859
_pd_proc_ls_prof_wR_factor       0.1282
_refine_ls_goodness_of_fit_all   1.49
_refine_ls_number_constraints    0
_refine_ls_number_parameters     21
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0441
_refine_ls_R_factor_gt           0.0312
_refine_ls_shift/su_max          0.0356
_refine_ls_shift/su_mean         0.0111
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_all         0.0404
_refine_ls_wR_factor_gt          0.0392
_cod_data_source_file            dq5016sup1.cif
_cod_data_source_block           II
_cod_depositor_comments
;
The following automatic conversions were performed:

'_diffrn_radiation_probe' value 'X-ray' changed to 'x-ray' according
to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/IUCr/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4268 2015-11-12 08:31:59Z antanas 

 Adding full bibliography for 2108027--2108028.cif.
;
_cod_original_cell_volume        206.967(4)
_cod_database_code               2108028
_cod_database_fobs_code          2108028